Journal of Colloid and Interface Science 456 (2015) 206–209
Contents lists available at ScienceDirect
Journal of Colloid and Interface Science journal homepage: www.elsevier.com/locate/jcis
Liposomes as nanoreactors for the photochemical synthesis of gold nanoparticles Sushanth Gudlur 1, Camilla Sandén, Petra Matoušková 2, Chiara Fasciani 3, Daniel Aili ⇑ Division of Molecular Physics, Department of Physics, Chemistry and Biology (IFM), Linköping University, SE-583 36 Linköping, Sweden
g r a p h i c a l a b s t r a c t
Photochemical synthesis of gold nanoparcles in bulk solvent (top panel) and within liposomes (boom panel)
a r t i c l e
i n f o
Article history: Received 13 May 2015 Revised 22 June 2015 Accepted 22 June 2015 Available online 24 June 2015
a b s t r a c t A simple and novel method for the photochemical synthesis of AuNPs in liposomes is described. Gold salt is co-encapsulated with the photoinitiator Irgacure-2959 in POPC liposomes prepared via traditional thin-ﬁlm hydration technique. UVA irradiation for 15 min results in encapsulated AuNPs of 2.8 ± 1.6 nm in diameter that are primarily dispersed in the aqueous interior of the liposomes. Ó 2015 Elsevier Inc. All rights reserved.
Keywords: Liposomes AuNPs Nanoreactors
Gold nanoparticles (AuNPs) have widespread applications in plasmonics , biosensors , electronics , catalysis , ⇑ Corresponding author. E-mail address: [email protected] (D. Aili). Current address: Centre for Biomimetic Sensor Science, School of Materials Science and Engineering, Nanyang Technological University, Singapore 637553, Singapore. 2 Current address: Centre for Materials Research, Faculty of Chemistry, Brno University of Technology, Purkynova 118, 612 00 Brno, Czech Republic. 3 Current address: Istituto Italiano di Tecnologia, Viale Regina Elena 291, 00161 Rome, Italy. 1
http://dx.doi.org/10.1016/j.jcis.2015.06.033 0021-9797/Ó 2015 Elsevier Inc. All rights reserved.
imaging and drug delivery [5,6]. A large number of methods have been developed and optimized for synthesizing AuNPs with deﬁned sizes and shapes [7,8], and typically involves the chemical reduction of Au (III) to Au (0). The initial small clusters of reduced gold thus obtained serve as nucleation sites for the subsequent growth of nanoparticles. For synthesis of spherical AuNPs, besides a reducing agent, an additional stabilizing or capping agent is sometimes added to the reaction mixture to prevent the AuNPs from aggregating. McGilvray et al. , reported a simple and rapid photochemical synthesis of AuNPs to obtain monodisperse spherical nanoparticles that are stable in suspension. In this synthesis,
S. Gudlur et al. / Journal of Colloid and Interface Science 456 (2015) 206–209
the reduction of Au (III) was achieved by ketyl radicals generated due to the UVA-irradiation of Irgacure-2959 (Irg), a photoinitiator. Additionally, the 4-hydroxyethoxy benzoic acid generated from irradiated Irg eventually acts to stabilize the AuNPs and thus prevents them from aggregating. Liposomes are excellent candidates for the compartmentalized synthesis of AuNPs , especially if the end-applications are in the ﬁeld of biological probes and drug delivery. Such compartmentalized synthesis offers the possibility to: control particle size, control the environment of synthesis to include catalytically active components, and carry out synthesis in a highly organized solvent structure . Yet, despite such advantages, previous attempts at synthesizing AuNPs within liposomes have resulted in high size polydispersity, inhomogeneity in shape, or poor yield [12–14]. Recently, the synthesis of AuNPs within liposomes was achieved by the controlled diffusion of stabilizing agents into encapsulated gold salt solutions [15,16], or by doping the lipids that constitute a liposome with glycerol that acts as a reducing agent . However, these approaches have had the need to either modify the method of liposome preparation or use special lipids to achieve controlled synthesis of AuNPs. In this communication, we describe a simple method (Fig. 1) for the controlled synthesis of spherical AuNPs with an average size of 2.8 ± 1.6 nm, inside palmitoyl oleoyl phosphocholine (POPC) liposomes. The resulting AuNPs are homogeneous in size and shape. Moreover, this simple method circumvents the need for separating unencapsulated AuNPs after their synthesis, which can be challenging when employing the more traditional method of encapsulating preformed AuNPs within liposomes. All these, without having to (1) modify existing liposome preparation techniques, (2) introduce additional stabilizing agents in solution, or (3) dope/modify lipids that constitute a liposome, with reducing or stabilizing agents. A freshly prepared solution of HAuCl4 (0.1 mg/mL) and Irg (1 mM) in deionized water was encapsulated into POPC liposomes (2 mg/mL) obtained via the thin-ﬁlm hydration technique  followed by extrusion using a polycarbonate ﬁlter of 100 nm pore size. After removal of unencapsulated HAuCl4 and Irg by separating them over a Sephadex G-25 spin column, the samples were irradiated in a photoreactor with 108 lW/m2 UVA light (365 nm) for 15 min, to generate stable AuNPs within the conﬁnes of the liposome. Photochemical synthesis of AuNPs within liposomes was conﬁrmed by the presence of the localized surface plasmon resonance (LSPR) band centered around 530 nm (Fig. 2). While this LSPR band is typically centered around 520 nm for small (10 nm) and dispersed AuNPs, its position is affected by factors such as particle size, shape, refractive index of the medium, temperature and by species adsorbed on the nanoparticle surface . The position of the LSPR band for AuNPs within liposomes appears red shifted due to the presence of liposomes that scatter signiﬁcantly at lower wavelengths. The effect of liposome scattering on the LSPR peak position was conﬁrmed using liposome encapsulation of commercial AuNPs. In the absence of liposomes they show kmax at 520 nm, and when encapsulated, the peak shifted to kmax 550 nm (Fig. S1). On the other hand, very small AuNPs (<2 nm) lose their plasmonic properties and hence will not show an LSPR band [19–21]. This loss of plasmonic properties may explain to some extent, the relatively weaker LSPR band from samples where AuNPs were synthesized within liposomes. Interestingly, transmission electron microscopy (TEM) revealed signiﬁcant differences in nanoparticle size and the overall size distribution of the AuNPs synthesized within liposomes and in bulk solvent (Fig. 3) using otherwise identical conditions. The AuNPs synthesized within liposomes are very homogeneous in shape and size (Fig. 3A). Based on the TEMs and size distribution analysis
Fig. 1. Schematic illustration of the photochemical synthesis of AuNPs in bulk solvent (top panel) and within liposomes (bottom panel). Green circles represent liposomes and golden spheres represent AuNPs. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
Fig. 2. UV–Vis spectra of 0.1 mg/mL HAuCl4 + 1 mM Irg samples unencapsulated (gray lines) or encapsulated within POPC liposomes (black lines). Samples were prepared in the dark (dashed lines) followed by UVA-irradiation (IRR) for 15 min (solid lines) to initiate AuNP synthesis.
performed on these images, the AuNPs are spherical and have an average size of 2.8 ± 1.6 nm (Figs. 3A and 4A). In comparison, there is a signiﬁcant difference in the size range of AuNPs synthesized in bulk solvent when using the same conditions but excluding liposomes (Figs. 3B and 4A). These nanoparticles are signiﬁcantly larger in size and more polydispersed. The large difference in the AuNP sizes between those synthesized within liposomes and those in the bulk solvent is presumably due to an effect of conﬁnement as well as the presence of a lipid bilayer. The inner membrane of the liposome offers a convenient surface for adsorption, formation and growth of nuclei but affects the diffusion coefﬁcient of the nuclei [22,23]. Hence, when compared to the bulk solvent, the nuclei formation within the liposomes is fast but the smaller diffusion coefﬁcient of the nuclei along with the physical barrier which inhibits NP diffusion, encounter and agglomeration, slows down the rate of the particle growth . Such reduced growth rates allow for other processes such as the capping/stabilization of AuNPs to occur and thus limits and controls the size of the particles formed. We investigated the effect of HAuCl4 + Irg concentrations and time of irradiation on AuNP synthesis in suspension (Fig. S2). We
S. Gudlur et al. / Journal of Colloid and Interface Science 456 (2015) 206–209
Fig. 3. TEM characterization of AuNPs synthesized within POPC liposomes (A) or in bulk solvent (B). Insets are magniﬁed images from the same samples. Magniﬁcation in Inset A is a portion of the liposome. Colored inset in (A) is a representation of AuNPs within liposomes. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
chose the minimum concentration and time of irradiation required to synthesize stable AuNPs, for synthesis within POPC liposomes. This was done to avoid any effects of AuNP aggregation due to high concentration of reactants and lipid peroxidation due to excessive UVA irradiation. In the case of AuNPs synthesized within liposomes, from the TEMs alone, it is difﬁcult to ascertain the exact location of the AuNPs. Besides being localized within the aqueous region of the liposome, the AuNPs, to a lesser extent, are expected to be trapped both on the periphery (via electrostatic interaction) as well as within the bilayer. Lipid peroxidation is expected to contribute to some reduction within the bilayer or in its vicinity [13,14]. It is known that certain lipids are able to spontaneously reduce Au (III) to Au (0) through the oxidation of the –OH groups to –COOH groups . This type of reduction may explain the presence of a weak LSPR band in our liposome samples when the samples were prepared in the dark and in the absence of UVA-irradiation (Fig. 2, black-dashed line). The LSPR band is absent when control HAuCl4 solution containing Irg was prepared in the dark and not irradiated (Fig. 2, gray-dashed line). Additionally, the presence of Irg and the subsequent UVA-irradiation of the liposomes can induce an oxidative stress leading to some lipid peroxidation, which cannot be avoided given the photochemical method of this AuNP synthesis. From the TEMs (Fig. 3A), it can be seen that some AuNPs are present outside the liposomes. This is most likely due to a combination of (1) the diffusion of trace amounts of the gold from within the liposomes during the separation/puriﬁcation stage (2) due to normal liposomal leakage and/or (3) disruption of liposomes during TEM sample preparation. To investigate the effect of UV irradiation on the liposomes, samples were analyzed with dynamic light scattering (DLS). The
Fig. 4. (A) Size distribution analysis of particles synthesized with 0.1 mg/mL HAuCl4 + 1 mM Irg in bulk solvent (gray) where n = 231, and encapsulated in POPC liposomes (black) where n = 509. (B) DLS correlation curve for encapsulated samples prepared with 0.1 mg/mL HAuCl4 + 1 mM Irg before (gray) and after (black) UVA-irradiation. The inset shows size distribution obtained using the CONTIN algorithm. POPC liposomes retain their size to a large extent after irradiation.
DLS instrument consisted of a ALV-CGS-5022F Goniometer system, a HeNe laser and a dual multiple-tau digital correlator (ALV-6010-160). For each sample, the count rate was approximately 350 kHz with a measuring time of 10 30 s. Correlation curves and calculated size distributions were compared and showed little change for all liposome containing samples (Fig. 4B). The liposomes retain their size which is a good indication that they also retain their integrity.
Conclusion Taken together, these results indicate that it is possible to synthesize AuNPs of homogeneous size distribution within liposomes without the need to modify existing methods of liposome preparation. We envision that this method of AuNP synthesis can be extended to other methods of liposome preparation as well. While we have demonstrated the controlled synthesis of AuNPs in liposomes prepared from POPC, which are already in the liquid-crystalline state at room temperature, this can be potentially expanded to liposomes prepared with other phospholipids having different gel-to-crystalline phase transition temperatures. The choice of lipids will therefore dictate the stability and release pattern-which is an important trigger control when it comes to designing suitable drug delivery systems. AuNPs within liposomes have applications as probes in biological processes wherein, the course and fate of the liposomes within the cell or body can be followed over time. In the case of drug delivery, the release of the contents of such liposomes can be triggered by thermal ablation via plasmon excitation of AuNPs. While this method may not be
S. Gudlur et al. / Journal of Colloid and Interface Science 456 (2015) 206–209
suitable for all drugs or excipients being encapsulated in liposomes, because of the drug’s interaction with AuNPs or the drug’s stability toward UVA-irradiation, it can prove useful in many other instances. An alternative strategy to obtain liposome encapsulated AuNPs is by encapsulating pre-formed AuNPs into liposomes. Here, a thin ﬁlm of dried lipids is hydrated with pre-formed AuNPs in suspension. After extruding the liposomes, separation of unencapsulated AuNPs is achieved via size exclusion chromatography or centrifugation. Due to the small difference in their sizes (AuNPs and liposomes), size exclusion chromatography is challenging while centrifugation is time consuming. Using the method described in this communication, this step can be circumvented since the separation step is performed before the AuNPs are synthesized. Removing unencapsulated gold salt solution using Sephadex G-25 spin columns is both easier and faster than removing unencapsulated AuNPs.
Acknowledgements This work was supported by the Swedish Foundation for Strategic Research (SSF) and the Center for Integrative Regenerative Medicine (IGEN) at Linköping University. During this study C.S. was enrolled in the graduate school Forum Scientium. The authors thank Batika Saxena for creating the artwork.
Appendix A. Supplementary material Supplementary data associated with this article can be found, in the online version, at http://dx.doi.org/10.1016/j.jcis.2015.06.033.
References  C.J. Orendorff, T.K. Sau, C.J. Murphy, Small 2 (2006) 636.  S. Szunerits, R. Boukherroub, Chem. Commun. 48 (2012) 8999.  D. Huang, F. Liao, S. Molesa, D. Redinger, V. Subramanian, J. Electrochem. Soc. 150 (2003) G412.  B. Hvolbæk, T.V.W. Janssens, B.S. Clausen, H. Falsig, C.H. Christensen, J.K. Nørskov, Nano Today 2 (2007) 14.  T. Curry, R. Kopelman, M. Shilo, R. Popovtzer, Contrast Media Mol. Imaging 9 (2014) 53.  R.A. Sperling, P. Rivera Gil, F. Zhang, M. Zanella, W.J. Parak, Chem. Soc. Rev. 37 (2008) 1896.  P. Zhao, N. Li, D. Astruc, Coord. Chem. Rev. 257 (2013) 638.  M.C. Daniel, D. Astruc, Chem. Rev. 104 (2004) 293.  K.L. McGilvray, M.R. Decan, D. Wang, J.C. Scaiano, J. Am. Chem. Soc. 128 (2006) 15980.  P. He, M.W. Urban, Biomacromolecules 6 (2005) 1224.  D.G. Shchukin, G.B. Sukhorukov, Adv. Mater. 16 (2004) 671.  G.M. Chow, M.A. Markowitz, R. Rayne, D.N. Dunn, A. Singh, J. Colloid Interface Sci. 183 (1996) 135.  F.C. Meldrum, B.R. Heywood, S. Mann, J. Colloid Interface Sci. 161 (1993) 66.  O. Regev, R. Backov, C. Faure, Chem. Mater. 16 (2004) 5280.  T.K. Sau, A.S. Urban, S.K. Dondapati, M. Fedoruk, M.R. Horton, A.L. Rogach, F.D. Stefani, J.O. Rädler, J. Feldmann, Colloids Surf. A: Physicochem. Eng. Aspects 342 (2009) 92.  R. Genc, M. Ortiz, C. Sullivan, J. Nanopart. Res. 16 (2014) 1.  R. Genc, G. Clergeaud, M. Ortiz, C.K. O’Sullivan, Langmuir 27 (2011) 10894.  A.D. Bangham, R.W. Horne, J. Mol. Biol. 8 (1964) 660.  Z.Y. Li, J.P. Wilcoxon, F. Yin, Y. Chen, R.E. Palmer, R.L. Johnston, Faraday Discuss. 138 (2008) 363.  S. Gilb, K. Hartl, A. Kartouzian, J. Peter, U. Heiz, H. Boyen, P. Ziemann, Eur. Phys. J. D 45 (2007) 501.  H. Weissker, C. Mottet, Phys. Rev. B 84 (2011) 165443.  T.V. Liveri (Ed.), J. David Lockwood, 2006, p. 75 (Chapter 2).  M.T. Kennedy, B.A. Korgel, H.G. Monbouquette, J.A. Zasadzinski, Chem. Mater. 10 (1998) 2116.  C. Tojo, M.C. Blanco, F. Rivadulla, M.A. López-Quintela, Langmuir 13 (1997) 1970.  K. Esumi, T. Hosoya, A. Suzuki, K. Torigoe, Langmuir 16 (2000) 2978.
Target drug delivery methodology is becoming increasingly important to overcome the shortcomings of conventional drug delivery absorption method. It improves the action time with uniform distribution and poses minimum side effects, but is usually dif
Reactive and pharmaceutical-grade heparins were used as biologically compatible reducing and stabilizing agents to photochemically synthesize colloidal gold nanoparticles. Aggregates and anisotropic shapes were obtained photochemically under UV black
Gold-containing polymer nanotubes, which showed both catalytic activity and resistance to leaching, were prepared by the "tubes by fiber templates" (TUFT) process. For this purpose, electrospun polymer nonwovens with incorporated poly(L-lactide)-stab
Soluble conjugated polymeric nanoparticles are synthesized by Suzuki-type polycondensation of two monomers (Ax + By, x>2, y≥2) in the channel of ordered mesoporous silica-supported carbon nanomembranes (nanoreactors). These synthesized soluble conjug
DNA cross-linked hydrogel was used as a matrix for synthesis of gold nanoparticles. DNA possesses a strong affinity to transition metals such as gold, which allows for the concentration of Au precursor inside a hydrogel. Further reduction of HAuCl4 i
The shape of nanoparticles has been recognized as an important attribute that determines their applicability in various fields. The flower shape (F-shape) has been considered and is being focused on, because of its enhanced properties when compared t
Yolk-shell nanoparticles (YSNs) with active metal cores have shown promising applications in nanoreactors with excellent catalytic performance. In this work, Fe(0)@SiO2 YSNs were synthesized by a sequential "two-solvents" impregnation-reduction appro
Glyco-gold nanoparticles combine in a single entity the peculiar properties of gold nanoparticles with the biological activity of carbohydrates. The result is an exciting nanosystem, able to mimic the natural multivalent presentation of saccharide mo
In this report, we show how the classical and widely used Turkevich synthesis can be improved significantly by simple adjustments. The gold nanoparticles (AuNPs) produced with the optimized protocol have a much narrower size distribution (5-8% standa
Gold nanoparticles (GNPs) were prepared using four different plant extracts as reducing and stabilizing agents. The extracts were obtained from the following plants: Salvia officinalis, Lippia citriodora, Pelargonium graveolens and Punica granatum. T